one - dimensional ( 1d ) nanostructured magnesium salts with different morphologies , such as needle , rod , wire , tube , and belt , have attracted much attention because of their unique properties and potential applications in nanotechnical fields . up to now
much work has been focused on the control of the morphologies of 1d 513mos since it can be used as the reinforcing agent , the flame retardant , or as the precursor for the fabrication of 1d mgo or mg(oh)2[6 - 8 ] .
it was reported that the 513mos whisker agglomerates with a length of up to 200 m and a diameter of 0.81.2 m were formed using mgso4 and mg(oh)2 or mgo as the reactants .
the sector - like 513mos whiskers with a length of 2050 m and a diameter of 0.21.0 m were synthesized using mgso4 and naoh as the raw materials [ 11 - 13 ] .
dispersive 1d 513mos without agglomerates or the sector - like were formed by employing mgso4 or the mixture of mgso4 and mgcl2 as the magnesium source and the weak alkali nh4oh as the precipitation agent [ 14 - 16 ] . but little work has been reported on the control of the sizes ( length and diameter ) of the 1d 513mos and it is still a challenge to synthesize 1d 513mos with high aspect ratio and perfect uniformity . generally the solution with a lower supersaturation was favorable for the anisotropic or 1d growth of the crystals , which can be achieved by using dilute reactants or chelating agents .
for example , it was reported that the presence of edta can control the morphologies and sizes of the corresponding particles owing to the chelating effects of edta with ca , zn , ce , fe , co , and bi , which can change the forms of the aqueous ions , producing a solution with less free metal ions to control the crystals growth .
the growth habits of the crystals can also be altered by the capping effect of edta on the surfaces of the crystals . in the present work
the 513 mos nanowires with high aspect ratio were formed by precipitation of mgso4and nh4oh solutions at room temperature followed by treatment at hydrothermal conditions .
the supersaturations of the solutions were controlled at relatively low levels , which were achieved by controlling the mixing ways of the reactants or addition of edta .
the preferential orientation of 513mos nanowires was identified and the related process mechanisms were discussed .
commercial reagents ( nh4oh , mgso4  7h2o , and edta ) with analytical grade provided by beijing chemical regent factory were used in the experiments .
three ways were adapted for the formation of the precursor slurries at room temperature : ( 1 ) single injection : 35 ml of 1.01.5 mol lmgso4was dropped ( 3.0 ml min ) into 20 ml of 5.09.0 mol lnh4oh ; ( 2 ) double injection : 35 ml of 1.01.5 mol lmgso4and 20 ml 5.09.0 mol lnh4oh were dropped ( 3.0 ml min ) simultaneously into 510 ml water ; ( 3 ) single injection in the presence of edta : 35 ml of 1.01.5 mol lmgso4mixed with varying amount of edta was dropped ( 3.0 ml min ) into 20 ml of 59 mol lammonia .
the slurry formed at room temperature was then transferred to a teflon - lined stainless steel autoclave with an inner volume of 80 cm , heated ( 5 c min ) to 150 c and kept under isothermal condition for 8.012.0 h. the autoclave was cooled down to room temperature naturally after hydrothermal treatment and the product was filtrated , washed , and dried at 105 c for 12.0 h. the morphology and the microstructure of the samples were examined with the field emission scanning electron microscopy ( fesem , jsm 7401f , jeol , japan ) , the high - resolution transmission electron microscope ( hrtem , jem-2010 , jeol , japan ) and the selected area electron diffraction ( saed ) .
the crystallization and the composition of the samples were identified by the powder x - ray diffraction ( xrd , d / max2500 , rigaku , japan ) using cuk (  = 0.154178 nm ) radiation .
the concentrations of mgand so4were analyzed by edta titration and barium chromate spectrophotometry ( model 722 , xiaoguang , china ) , respectively .
commercial reagents ( nh4oh , mgso4  7h2o , and edta ) with analytical grade provided by beijing chemical regent factory were used in the experiments .
three ways were adapted for the formation of the precursor slurries at room temperature : ( 1 ) single injection : 35 ml of 1.01.5 mol lmgso4was dropped ( 3.0 ml min ) into 20 ml of 5.09.0 mol lnh4oh ; ( 2 ) double injection : 35 ml of 1.01.5 mol lmgso4and 20 ml 5.09.0 mol lnh4oh were dropped ( 3.0 ml min ) simultaneously into 510 ml water ; ( 3 ) single injection in the presence of edta : 35 ml of 1.01.5 mol lmgso4mixed with varying amount of edta was dropped ( 3.0 ml min ) into 20 ml of 59 mol lammonia .
the slurry formed at room temperature was then transferred to a teflon - lined stainless steel autoclave with an inner volume of 80 cm , heated ( 5 c min ) to 150 c and kept under isothermal condition for 8.012.0 h. the autoclave was cooled down to room temperature naturally after hydrothermal treatment and the product was filtrated , washed , and dried at 105 c for 12.0 h.
the morphology and the microstructure of the samples were examined with the field emission scanning electron microscopy ( fesem , jsm 7401f , jeol , japan ) , the high - resolution transmission electron microscope ( hrtem , jem-2010 , jeol , japan ) and the selected area electron diffraction ( saed ) .
the crystallization and the composition of the samples were identified by the powder x - ray diffraction ( xrd , d / max2500 , rigaku , japan ) using cuk (  = 0.154178 nm ) radiation .
the concentrations of mgand so4were analyzed by edta titration and barium chromate spectrophotometry ( model 722 , xiaoguang , china ) , respectively .
figure 1shows the influence of the preparation ways of the precursors on the morphologies of the hydrothermal products .
1d product with a length of 2030 m and an ununiform diameter of 0.3 1.7 m were prepared via the single injection route ( fig .
uniform nanowires with a length to 2060 m and a diameter of 60300 nm were fabricated in the case of the double injection route ( fig .
1b ) , which may be connected with the decrease of the supersaturation of 513mos in the solution due to the dilution of the reactants and will be discussed in detail later .
the morphologies of the products prepared via single injection ( a ) and double injection ( b ) the influence of edta on the morphologies of the hydrothermal products was shown in fig .
2 . 1d product with a length of 3050 m and a diameter of 0.21 m were formed at 1.0  10 mol ledta ( fig .
2b , c ) as the edta concentration increased up to 1.0  10 mol l. the clusters of the products were composed of the twisted nanowires with a length of 100200 m and an aspect ratio up to 1,000 .
the diameter of the product was broadened to 0.150.6 m and the length was about 100 m in the case of 1.0  10 mol ledta ( fig .
influence of edta concentrations on the morphologies of the products ( a ) 1.0  10 mol l ; ( b , c ) ( different magnifications ) 1.0  10 mol l ; ( d ) 1.0  10 mol l figure 3shows the xrd patterns of the hydrothermal products formed in presence of edta .
all the diffraction peaks can be indexed as those of the orthorhombic 5mg(oh)2  mgso4  3h2o ( pdf no .
the gradual increase of the diffraction intensities with the increase of edta concentration indicated that the presence of edta was favorable for the crystallization of 1d 513 mos .
it was also noticed that most of the xrd peaks were attributed to ( ) planes , indicating that the 513mos nanowires may have a preferential growth along b axis owing to its inherent structure .
2 the hrtem image and the saed pattern of the 513mos nanowires prepared in the presence of 1.0  10 mol ledta were shown in fig .
4 . the interplanar distances of the lattice fringes parallel ( fig . 4b , corresponding to the rectangular part of the nanowire in fig .
4c , corresponding to the trigonal part of the nanowire in fig .4a ) to the growth direction of the whiskers were 5.1 and 2.25  , quite similar to the spacing of ( 202 ) plane ( d ( 202 ) = 5.12  ) and ( 114 ) plane ( d ( 114 ) = 2.255  ) , respectively , indicating the preferential orientation of the nanowires along the   direction , which was reconfirmed by the saed analysis in fig . 4d and also identical with the xrd analysis shown in fig .
3 . tem ( a ) , hrtem images ( b , c ) and saed pattern ( d ) of 513mos nanowire figure 5 shows the influence of the preparation ways of the mg(oh)2 precursors on the variation of [ mg and the supersaturation of 513mos with the hydrothermal time . the supersaturation of 513mos was presented by [ mg[so4[oh according to the following formation reaction:(1 ) variations of [ mg ] ( a ) and super - saturation of 513os ( b ) with hydrothermal time .
preparation ways of mg(oh)2precursor : a  single injection without edta , b  double injection without edta , c  single injection with 1.0  10 mol ledta the presence of edta led to the decrease of [ mg ] ( fig . 5a ) and the supersaturation of 513mos ( fig .
5b ) , which may be connected with the chelating and/or the capping effects of edta .
the slow release of mgfrom the complexes might be favorable for the 1d growth of 513mos .
the varying binding abilities of edta on different planes may also inhibit the radial growth and promote the axial growth of the 513mos nanowires .
the increase of [ mg ] and the supersaturation of 513mos within initial 8 h of reaction should be attributed mainly to the dissolution of the mg(oh)2precursor , and the decrease of [ mg ] and the supersaturation of 513mos after 610
the lower supersaturations of 513mos achieved in either the double injection route or in the presence of minor amount of edta were favorable for the formation of 513mos nanowires with high aspect ratio .
513mos nanowires with a length of 2060 m and a diameter of 60300 nm were synthesized via the double injection - hydrothermal reaction and the uniform 513mos nanowires with a length of 100200 m and a diameter of 80200 nm were formed via single injection edta - assisted hydrothermal reaction route .
the lower supersaturations of 513mos achieved in either the double injection route or in the presence of minor amount of edta , were favorable for the preferential growth of 513mos along b axis , leading to the formation of 513mos nanowires with high aspect ratios .
this work is supported by the national natural science foundation of china ( no.50574051 ) .
 one - dimensional magnesium oxysulfate 5mg(oh)2  mgso4  3h2o ( abbreviated as 513mos ) with high aspect ratio has attracted much attention because of its distinctive properties from those of the conventional bulk materials . 
 513mos nanowires with different morphologies were formed by varying the mixing ways of mgso4  7h2o and nh4oh solutions at room temperature followed by hydrothermal treatment of the slurries at 150 c for 12 h with or without edta . 
 513mos nanowires with a length of 2060 m and a diameter of 60300 nm were prepared in the case of double injection ( adding mgso4  7h2o and nh4oh solutions simultaneously into water ) , compared with the 513mos with a length of 2030 m and a diameter of 0.31.7 m in the case of the single injection ( adding mgso4  7h2o solution into nh4oh solution ) . 
 the presence of minor amount of edta in the single injection method led to the formation of 513mos nanowires with a length of 100200 m , a diameter of 80200 nm , and an aspect ratio of up to 1000 . 
 the analysis of the experimental results indicated that the hydrothermal solutions with a lower supersaturation were favorable for the preferential growth of 513mos nanowires along b axis . 